#------------------------------------------------------------------------------
#$Date: 2024-07-05 16:09:27 +0200 (Fri 05 de Jul de 2024) $
#$Revision: 292872 $
#$URL: svn://www.crystallography.net/cod/cif/1/57/15/1571504.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1571504
loop_
_publ_author_name
'Yan, Mei'
'Hu, Chun-Li'
'Tang, Ru-Ling'
'Yao, Wen-Dong'
'Liu, Wenlong'
'Guo, Sheng-Ping'
_publ_section_title
;
 KBa₃M₂F₁₄Cl (M = Zr, Hf): novel
 short-wavelength mixed metal halides with the largest second-harmonic
 generation responses contributed by mixed functional moieties.
;
_journal_issue                   22
_journal_name_full               'Chemical science'
_journal_page_first              8500
_journal_page_last               8505
_journal_paper_doi               10.1039/d4sc01259c
_journal_volume                  15
_journal_year                    2024
_chemical_formula_moiety         'Ba3 Cl F14 Hf2 K'
_chemical_formula_sum            'Ba3 Cl F14 Hf2 K'
_chemical_formula_weight         1109.55
_chemical_name_systematic        KBa3Hf2F14Cl
_space_group_crystal_system      tetragonal
_space_group_IT_number           115
_space_group_name_Hall           'P -4 -2'
_space_group_name_H-M_alt        'P -4 m 2'
_atom_sites_solution_primary     dual
_audit_creation_date             2024-04-06
_audit_creation_method
;
Olex2 1.5
(compiled 2021.08.20 svn.r13c46975 for OlexSys, GUI svn.r6405)
;
_audit_update_record
;
2024-04-09 deposited with the CCDC.	2024-04-30 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   5.7439(3)
_cell_length_b                   5.7439(3)
_cell_length_c                   10.2541(7)
_cell_measurement_reflns_used    2177
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.41
_cell_measurement_theta_min      3.55
_cell_volume                     338.31(3)
_computing_cell_refinement       'SAINT V8.40A (Bruker, 2019)'
_computing_data_collection       'SAINT V8.40A (Bruker, 2019)'
_computing_data_reduction        'SAINT V8.40A (Bruker, 2019)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2014/7 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0385
_diffrn_reflns_av_unetI/netI     0.0263
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            2574
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.412
_diffrn_reflns_theta_min         1.986
_diffrn_source_current           1.0
_diffrn_source_power             0.05
_diffrn_source_voltage           50.0
_exptl_absorpt_coefficient_mu    24.534
_exptl_absorpt_correction_T_max  0.3331
_exptl_absorpt_correction_T_min  0.1621
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1402 before and 0.0551 after correction.
The Ratio of minimum to maximum transmission is 0.4866.
The λ/2 correction factor is Not present.
;
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    5.446
_exptl_crystal_description       block
_exptl_crystal_F_000             474
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.07
_refine_diff_density_max         0.946
_refine_diff_density_min         -0.846
_refine_diff_density_rms         0.146
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.03(3)
_refine_ls_extinction_coef       0.0365(12)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.091
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     36
_refine_ls_number_reflns         469
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.091
_refine_ls_R_factor_all          0.0139
_refine_ls_R_factor_gt           0.0134
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+0.0095P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0292
_refine_ls_wR_factor_ref         0.0293
_reflns_Friedel_coverage         0.686
_reflns_Friedel_fraction_full    0.993
_reflns_Friedel_fraction_max     0.995
_reflns_number_gt                459
_reflns_number_total             469
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d4sc01259c2.cif
_cod_data_source_block           1_CCDC1
_cod_depositor_comments
'Adding full bibliography for 1571503--1571504.cif.'
_cod_original_cell_volume        338.31(4)
_cod_database_code               1571504
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.279
_shelx_estimated_absorpt_t_min   0.067
_olex2_refinement_description
;
1. Twinned data refinement
 Scales: 0.97(3)
 0.03(3)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'y, -x, -z'
'-y, x, -z'
'x, -y, z'
'-x, y, z'
'y, x, -z'
'-y, -x, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Hf1 Hf 0.0000 0.5000 0.75599(3) 0.00899(15) Uani 1 4 d S T P . .
Ba2 Ba 0.0000 1.0000 1.0000 0.0121(3) Uani 1 8 d S T P . .
Ba1 Ba 0.0000 0.5000 0.36729(5) 0.01955(18) Uani 1 4 d S T P . .
K1 K 0.5000 0.5000 1.0000 0.0150(9) Uani 1 8 d S T P . .
F1 F -0.2205(8) 0.5000 0.6021(4) 0.0223(11) Uani 1 2 d S T P . .
F2 F 0.2316(5) 0.7564(5) 0.8064(2) 0.0183(6) Uani 1 1 d . . . . .
Cl1 Cl 0.0000 0.0000 0.5000 0.0189(9) Uani 1 8 d S T P . .
F3 F 0.0000 0.5000 0.9630(4) 0.0187(13) Uani 1 4 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Hf Hf -0.5830 6.1852 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ba2 Hf1 Ba2 97.873(9) . 1_545 ?
Ba2 Hf1 Ba1 131.063(4) . . ?
Ba2 Hf1 Ba1 131.063(4) 1_545 . ?
Ba2 Hf1 K1 64.437(5) . 1_455 ?
K1 Hf1 Ba2 64.437(5) . . ?
K1 Hf1 Ba2 64.437(5) 1_455 1_545 ?
K1 Hf1 Ba2 64.437(5) . 1_545 ?
K1 Hf1 Ba1 131.063(4) 1_455 . ?
K1 Hf1 Ba1 131.063(4) . . ?
K1 Hf1 K1 97.873(9) . 1_455 ?
F1 Hf1 Ba2 120.81(6) . . ?
F1 Hf1 Ba2 120.81(6) 2_565 . ?
F1 Hf1 Ba2 120.81(6) . 1_545 ?
F1 Hf1 Ba2 120.81(6) 2_565 1_545 ?
F1 Hf1 Ba1 38.76(13) 2_565 . ?
F1 Hf1 Ba1 38.76(13) . . ?
F1 Hf1 K1 92.30(13) . 1_455 ?
F1 Hf1 K1 92.30(13) 2_565 . ?
F1 Hf1 K1 169.82(13) 2_565 1_455 ?
F1 Hf1 K1 169.82(13) . . ?
F1 Hf1 F1 77.5(3) . 2_565 ?
F1 Hf1 F2 127.06(9) 2_565 6 ?
F1 Hf1 F2 77.90(12) 2_565 5_565 ?
F1 Hf1 F2 127.06(9) 2_565 2_565 ?
F1 Hf1 F2 127.06(9) . . ?
F1 Hf1 F2 77.90(12) 2_565 . ?
F1 Hf1 F2 127.06(9) . 5_565 ?
F1 Hf1 F2 77.90(12) . 6 ?
F1 Hf1 F2 77.90(12) . 2_565 ?
F1 Hf1 F3 141.24(13) . . ?
F1 Hf1 F3 141.24(13) 2_565 . ?
F2 Hf1 Ba2 112.08(8) . 1_545 ?
F2 Hf1 Ba2 112.08(8) 2_565 . ?
F2 Hf1 Ba2 45.01(8) 6 . ?
F2 Hf1 Ba2 45.01(8) . . ?
F2 Hf1 Ba2 45.01(8) 2_565 1_545 ?
F2 Hf1 Ba2 112.08(8) 5_565 . ?
F2 Hf1 Ba2 45.01(8) 5_565 1_545 ?
F2 Hf1 Ba2 112.08(8) 6 1_545 ?
F2 Hf1 Ba1 104.60(7) 5_565 . ?
F2 Hf1 Ba1 104.60(7) . . ?
F2 Hf1 Ba1 104.60(7) 6 . ?
F2 Hf1 Ba1 104.60(7) 2_565 . ?
F2 Hf1 K1 108.88(7) 6 . ?
F2 Hf1 K1 49.11(8) 6 1_455 ?
F2 Hf1 K1 49.10(8) . . ?
F2 Hf1 K1 108.88(7) . 1_455 ?
F2 Hf1 K1 49.11(8) 2_565 1_455 ?
F2 Hf1 K1 49.11(8) 5_565 . ?
F2 Hf1 K1 108.88(7) 5_565 1_455 ?
F2 Hf1 K1 108.88(7) 2_565 . ?
F2 Hf1 F2 150.80(14) . 2_565 ?
F2 Hf1 F2 80.89(18) 2_565 5_565 ?
F2 Hf1 F2 91.80(18) . 5_565 ?
F2 Hf1 F2 80.89(18) . 6 ?
F2 Hf1 F2 150.80(14) 6 5_565 ?
F2 Hf1 F2 91.80(18) 2_565 6 ?
F2 Hf1 F3 75.40(7) 6 . ?
F2 Hf1 F3 75.40(7) . . ?
F2 Hf1 F3 75.40(7) 2_565 . ?
F2 Hf1 F3 75.40(7) 5_565 . ?
F3 Hf1 Ba2 48.937(4) . . ?
F3 Hf1 Ba2 48.937(4) . 1_545 ?
F3 Hf1 Ba1 180.0 . . ?
F3 Hf1 K1 48.937(4) . . ?
F3 Hf1 K1 48.937(4) . 1_455 ?
F2 Ba2 F2 57.42(11) . 6 ?
F2 Ba2 F2 120.93(7) 4_667 2_575 ?
F2 Ba2 F2 177.98(12) 8_667 2_575 ?
F2 Ba2 F2 120.93(7) 2_575 3_467 ?
F2 Ba2 F2 60.70(12) 4_667 7_467 ?
F2 Ba2 F2 120.93(7) 7_467 5_575 ?
F2 Ba2 F2 91.63(12) 6 3_467 ?
F2 Ba2 F2 91.63(12) 4_667 5_575 ?
F2 Ba2 F2 60.70(12) . 5_575 ?
F2 Ba2 F2 177.98(12) . 7_467 ?
F2 Ba2 F2 91.63(12) . 8_667 ?
F2 Ba2 F2 60.70(12) 8_667 3_467 ?
F2 Ba2 F2 120.93(7) 6 8_667 ?
F2 Ba2 F2 120.93(7) 6 7_467 ?
F2 Ba2 F2 57.42(11) 7_467 3_467 ?
F2 Ba2 F2 88.40(12) . 2_575 ?
F2 Ba2 F2 177.98(12) 6 4_667 ?
F2 Ba2 F2 57.42(11) 4_667 8_667 ?
F2 Ba2 F2 60.70(12) 6 2_575 ?
F2 Ba2 F2 88.40(12) 4_667 3_467 ?
F2 Ba2 F2 88.40(12) 8_667 7_467 ?
F2 Ba2 F2 120.93(7) . 4_667 ?
F2 Ba2 F2 177.98(12) 5_575 3_467 ?
F2 Ba2 F2 88.40(12) 6 5_575 ?
F2 Ba2 F2 120.93(7) . 3_467 ?
F2 Ba2 F2 120.93(7) 8_667 5_575 ?
F2 Ba2 F2 91.63(12) 7_467 2_575 ?
F2 Ba2 F2 57.42(11) 2_575 5_575 ?
F2 Ba2 F3 67.53(10) . 3_567 ?
F2 Ba2 F3 124.76(9) 8_667 1_565 ?
F2 Ba2 F3 53.49(9) 3_467 3_467 ?
F2 Ba2 F3 67.53(9) 4_667 1_565 ?
F2 Ba2 F3 124.76(9) 3_467 1_565 ?
F2 Ba2 F3 114.02(10) 5_575 . ?
F2 Ba2 F3 53.49(9) 7_467 3_467 ?
F2 Ba2 F3 124.76(9) . 3_467 ?
F2 Ba2 F3 67.53(10) 7_467 1_565 ?
F2 Ba2 F3 53.49(9) 5_575 1_565 ?
F2 Ba2 F3 53.49(9) 4_667 3_567 ?
F2 Ba2 F3 124.76(9) 7_467 . ?
F2 Ba2 F3 124.76(9) 5_575 3_467 ?
F2 Ba2 F3 124.76(9) 4_667 . ?
F2 Ba2 F3 67.53(10) 2_575 3_467 ?
F2 Ba2 F3 114.02(10) 6 1_565 ?
F2 Ba2 F3 67.53(10) 6 3_467 ?
F2 Ba2 F3 114.02(10) 7_467 3_567 ?
F2 Ba2 F3 53.49(9) 2_575 1_565 ?
F2 Ba2 F3 114.02(10) 4_667 3_467 ?
F2 Ba2 F3 114.02(10) 8_667 3_467 ?
F2 Ba2 F3 124.76(9) 2_575 3_567 ?
F2 Ba2 F3 53.49(9) . . ?
F2 Ba2 F3 53.49(9) 6 . ?
F2 Ba2 F3 114.02(10) 3_467 3_567 ?
F2 Ba2 F3 114.02(10) 2_575 . ?
F2 Ba2 F3 53.49(9) 8_667 3_567 ?
F2 Ba2 F3 67.53(10) 3_467 . ?
F2 Ba2 F3 124.76(9) 6 3_567 ?
F2 Ba2 F3 67.53(9) 8_667 . ?
F2 Ba2 F3 114.02(10) . 1_565 ?
F2 Ba2 F3 67.53(10) 5_575 3_567 ?
F3 Ba2 F3 90.98(2) 3_567 1_565 ?
F3 Ba2 F3 164.94(17) 1_565 . ?
F3 Ba2 F3 90.98(2) 3_467 . ?
F3 Ba2 F3 90.98(2) 3_467 1_565 ?
F3 Ba2 F3 90.98(2) 3_567 . ?
F3 Ba2 F3 164.94(17) 3_567 3_467 ?
F1 Ba1 F1 60.76(13) . 4_566 ?
F1 Ba1 F1 108.70(10) . 4_666 ?
F1 Ba1 F1 120.67(14) 4_666 4_566 ?
F1 Ba1 F1 108.70(10) . 3_556 ?
F1 Ba1 F1 120.67(14) 3_456 3_556 ?
F1 Ba1 F1 58.12(14) 3_456 4_566 ?
F1 Ba1 F1 108.70(10) 2_565 4_566 ?
F1 Ba1 F1 55.49(18) 2_565 . ?
F1 Ba1 F1 169.11(15) 3_556 4_566 ?
F1 Ba1 F1 58.12(14) 4_666 3_556 ?
F1 Ba1 F1 60.76(13) . 3_456 ?
F1 Ba1 F1 108.70(10) 2_565 3_456 ?
F1 Ba1 F1 60.76(13) 2_565 3_556 ?
F1 Ba1 F1 169.11(15) 4_666 3_456 ?
F1 Ba1 F1 60.76(13) 2_565 4_666 ?
F1 Ba1 F2 144.40(6) 2_565 3_466 ?
F1 Ba1 F2 109.73(9) . 7_456 ?
F1 Ba1 F2 144.40(6) . 4_656 ?
F1 Ba1 F2 109.73(9) . 3_466 ?
F1 Ba1 F2 109.73(9) 2_565 4_656 ?
F1 Ba1 F2 144.40(6) . 8_666 ?
F1 Ba1 F2 109.73(9) 2_565 8_666 ?
F1 Ba1 F2 144.40(6) 2_565 7_456 ?
F1 Ba1 Cl1 67.73(2) . . ?
F1 Ba1 Cl1 67.73(2) . 1_565 ?
F1 Ba1 Cl1 67.73(2) 2_565 . ?
F1 Ba1 Cl1 67.73(2) 2_565 1_565 ?
F2 Ba1 F1 141.15(9) 8_666 3_456 ?
F2 Ba1 F1 103.42(9) 4_656 3_456 ?
F2 Ba1 F1 141.15(9) 3_466 3_556 ?
F2 Ba1 F1 141.15(9) 7_456 4_666 ?
F2 Ba1 F1 49.05(9) 8_666 4_666 ?
F2 Ba1 F1 49.05(9) 7_456 3_456 ?
F2 Ba1 F1 83.75(10) 7_456 4_566 ?
F2 Ba1 F1 49.05(9) 3_466 4_566 ?
F2 Ba1 F1 103.42(9) 8_666 4_566 ?
F2 Ba1 F1 83.75(10) 8_666 3_556 ?
F2 Ba1 F1 83.75(10) 3_466 3_456 ?
F2 Ba1 F1 141.15(9) 4_656 4_566 ?
F2 Ba1 F1 83.75(10) 4_656 4_666 ?
F2 Ba1 F1 49.05(9) 4_656 3_556 ?
F2 Ba1 F1 103.42(9) 7_456 3_556 ?
F2 Ba1 F1 103.42(9) 3_466 4_666 ?
F2 Ba1 F2 98.91(10) 7_456 8_666 ?
F2 Ba1 F2 68.48(13) 7_456 3_466 ?
F2 Ba1 F2 61.43(12) 3_466 8_666 ?
F2 Ba1 F2 98.91(10) 4_656 3_466 ?
F2 Ba1 F2 61.43(12) 7_456 4_656 ?
F2 Ba1 F2 68.48(13) 4_656 8_666 ?
F2 Ba1 Cl1 76.69(6) 4_656 . ?
F2 Ba1 Cl1 76.69(6) 7_456 . ?
F2 Ba1 Cl1 141.89(7) 7_456 1_565 ?
F2 Ba1 Cl1 141.89(7) 3_466 . ?
F2 Ba1 Cl1 76.69(6) 8_666 1_565 ?
F2 Ba1 Cl1 141.89(7) 8_666 . ?
F2 Ba1 Cl1 141.89(7) 4_656 1_565 ?
F2 Ba1 Cl1 76.69(6) 3_466 1_565 ?
Cl1 Ba1 F1 113.47(7) 1_565 3_456 ?
Cl1 Ba1 F1 61.34(7) 1_565 4_566 ?
Cl1 Ba1 F1 113.47(7) . 4_566 ?
Cl1 Ba1 F1 113.47(7) . 4_666 ?
Cl1 Ba1 F1 61.34(7) 1_565 4_666 ?
Cl1 Ba1 F1 61.34(7) . 3_456 ?
Cl1 Ba1 F1 61.34(7) . 3_556 ?
Cl1 Ba1 F1 113.47(7) 1_565 3_556 ?
Cl1 Ba1 Cl1 129.295(18) 1_565 . ?
F2 K1 F2 117.67(6) 7_557 6_655 ?
F2 K1 F2 63.91(11) 3_567 7_557 ?
F2 K1 F2 94.08(11) 5_565 6_655 ?
F2 K1 F2 117.67(6) 5_565 8_667 ?
F2 K1 F2 178.08(11) 8_667 2_665 ?
F2 K1 F2 178.08(11) 5_565 3_567 ?
F2 K1 F2 117.67(6) 5_565 7_557 ?
F2 K1 F2 63.91(11) 5_565 2_665 ?
F2 K1 F2 63.91(11) 8_667 4_657 ?
F2 K1 F2 117.67(6) 8_667 6_655 ?
F2 K1 F2 178.08(11) 6_655 4_657 ?
F2 K1 F2 85.95(11) 5_565 4_657 ?
F2 K1 F2 85.95(11) 3_567 6_655 ?
F2 K1 F2 60.73(11) 2_665 6_655 ?
F2 K1 F2 85.95(11) . 8_667 ?
F2 K1 F2 117.67(6) 2_665 4_657 ?
F2 K1 F2 94.08(11) . 2_665 ?
F2 K1 F2 94.08(11) 8_667 7_557 ?
F2 K1 F2 117.67(6) 3_567 2_665 ?
F2 K1 F2 178.08(11) . 7_557 ?
F2 K1 F2 85.95(11) 7_557 2_665 ?
F2 K1 F2 117.67(6) . 4_657 ?
F2 K1 F2 63.91(11) . 6_655 ?
F2 K1 F2 94.08(11) 3_567 4_657 ?
F2 K1 F2 60.73(11) . 5_565 ?
F2 K1 F2 60.73(11) 7_557 4_657 ?
F2 K1 F2 117.67(6) . 3_567 ?
F2 K1 F2 60.73(11) 3_567 8_667 ?
F3 K1 F2 115.81(9) 3_557 3_567 ?
F3 K1 F2 115.81(9) 3_557 8_667 ?
F3 K1 F2 115.81(9) 1_655 . ?
F3 K1 F2 115.81(9) 1_655 5_565 ?
F3 K1 F2 126.19(8) . 3_567 ?
F3 K1 F2 115.81(9) . 6_655 ?
F3 K1 F2 115.81(9) 3_567 7_557 ?
F3 K1 F2 52.12(9) 3_567 8_667 ?
F3 K1 F2 65.68(9) 3_567 6_655 ?
F3 K1 F2 126.19(8) 3_557 6_655 ?
F3 K1 F2 52.12(9) 3_557 7_557 ?
F3 K1 F2 126.19(8) . 7_557 ?
F3 K1 F2 126.19(8) 1_655 8_667 ?
F3 K1 F2 52.12(9) 1_655 2_665 ?
F3 K1 F2 65.68(9) . 4_657 ?
F3 K1 F2 65.68(9) 3_557 5_565 ?
F3 K1 F2 115.81(9) . 2_665 ?
F3 K1 F2 115.81(9) 3_567 4_657 ?
F3 K1 F2 52.12(9) . 5_565 ?
F3 K1 F2 126.19(8) 1_655 4_657 ?
F3 K1 F2 52.12(9) 3_567 3_567 ?
F3 K1 F2 65.68(9) 3_557 2_665 ?
F3 K1 F2 52.12(9) . . ?
F3 K1 F2 52.12(9) 1_655 6_655 ?
F3 K1 F2 65.68(9) 3_567 . ?
F3 K1 F2 126.19(8) 3_557 . ?
F3 K1 F2 65.68(9) 1_655 3_567 ?
F3 K1 F2 65.68(9) . 8_667 ?
F3 K1 F2 126.19(8) 3_567 2_665 ?
F3 K1 F2 52.12(9) 3_557 4_657 ?
F3 K1 F2 126.19(8) 3_567 5_565 ?
F3 K1 F2 65.68(9) 1_655 7_557 ?
F3 K1 F3 90.98(2) 3_557 1_655 ?
F3 K1 F3 90.98(2) 3_567 1_655 ?
F3 K1 F3 164.94(17) 3_567 3_557 ?
F3 K1 F3 90.98(2) 3_567 . ?
F3 K1 F3 164.94(17) 1_655 . ?
F3 K1 F3 90.98(2) 3_557 . ?
Hf1 F1 Ba1 103.30(9) . 3_456 ?
Hf1 F1 Ba1 113.50(19) . . ?
Hf1 F1 Ba1 103.30(9) . 3_466 ?
Ba1 F1 Ba1 108.06(8) . 3_456 ?
Ba1 F1 Ba1 120.67(14) 3_456 3_466 ?
Ba1 F1 Ba1 108.06(8) . 3_466 ?
Hf1 F2 Ba2 103.41(11) . . ?
Hf1 F2 Ba1 124.61(10) . 3_566 ?
Hf1 F2 K1 98.75(11) . . ?
Ba2 F2 K1 91.21(7) . . ?
Ba1 F2 Ba2 118.57(11) 3_566 . ?
Ba1 F2 K1 113.79(10) 3_566 . ?
Ba1 Cl1 Ba1 100.565(7) . 3_556 ?
Ba1 Cl1 Ba1 129.294(17) . 1_545 ?
Ba1 Cl1 Ba1 129.294(18) 3_556 3_456 ?
Ba1 Cl1 Ba1 100.565(7) . 3_456 ?
Ba1 Cl1 Ba1 100.565(7) 3_556 1_545 ?
Ba1 Cl1 Ba1 100.565(7) 1_545 3_456 ?
Hf1 F3 Ba2 97.53(9) . 1_545 ?
Hf1 F3 Ba2 97.53(9) . . ?
Hf1 F3 K1 97.53(9) . 1_455 ?
Hf1 F3 K1 97.53(9) . . ?
Ba2 F3 Ba2 164.94(17) . 1_545 ?
Ba2 F3 K1 89.02(2) . 1_455 ?
K1 F3 Ba2 89.02(2) . 1_545 ?
K1 F3 Ba2 89.02(2) . . ?
K1 F3 Ba2 89.02(2) 1_455 1_545 ?
K1 F3 K1 164.94(17) . 1_455 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Hf1 Ba2 3.8090(3) 1_545 ?
Hf1 Ba2 3.8090(3) . ?
Hf1 Ba1 3.9857(6) . ?
Hf1 K1 3.8090(3) . ?
Hf1 K1 3.8090(3) 1_455 ?
Hf1 F1 2.023(4) . ?
Hf1 F1 2.023(4) 2_565 ?
Hf1 F2 2.051(3) 2_565 ?
Hf1 F2 2.051(3) 5_565 ?
Hf1 F2 2.051(3) 6 ?
Hf1 F2 2.051(3) . ?
Hf1 F3 2.123(4) . ?
Ba2 F2 2.769(3) 2_575 ?
Ba2 F2 2.769(3) 7_467 ?
Ba2 F2 2.769(3) 4_667 ?
Ba2 F2 2.769(3) 8_667 ?
Ba2 F2 2.769(3) 6 ?
Ba2 F2 2.769(3) 5_575 ?
Ba2 F2 2.769(3) . ?
Ba2 F2 2.769(3) 3_467 ?
Ba2 F3 2.8969(6) 3_567 ?
Ba2 F3 2.8969(6) 1_565 ?
Ba2 F3 2.8969(6) 3_467 ?
Ba2 F3 2.8969(6) . ?
Ba1 F1 3.305(2) 4_666 ?
Ba1 F1 2.721(4) . ?
Ba1 F1 3.305(2) 3_556 ?
Ba1 F1 3.305(2) 3_456 ?
Ba1 F1 3.305(2) 4_566 ?
Ba1 F1 2.721(4) 2_565 ?
Ba1 F2 2.740(3) 8_666 ?
Ba1 F2 2.740(3) 4_656 ?
Ba1 F2 2.740(3) 3_466 ?
Ba1 F2 2.740(3) 7_456 ?
Ba1 Cl1 3.1780(3) . ?
Ba1 Cl1 3.1780(3) 1_565 ?
K1 F2 2.913(3) 7_557 ?
K1 F2 2.913(3) 5_565 ?
K1 F2 2.913(3) 3_567 ?
K1 F2 2.913(3) . ?
K1 F2 2.913(3) 4_657 ?
K1 F2 2.913(3) 6_655 ?
K1 F2 2.913(3) 2_665 ?
K1 F2 2.913(3) 8_667 ?
K1 F3 2.8969(6) . ?
K1 F3 2.8969(6) 3_557 ?
K1 F3 2.8969(6) 1_655 ?
K1 F3 2.8969(6) 3_567 ?
F1 Ba1 3.305(2) 3_456 ?
F1 Ba1 3.305(2) 3_466 ?
F2 Ba1 2.740(3) 3_566 ?
Cl1 Ba1 3.1780(3) 1_545 ?
Cl1 Ba1 3.1780(3) 3_456 ?
Cl1 Ba1 3.1780(3) 3_556 ?
F3 Ba2 2.8969(6) 1_545 ?
F3 K1 2.8969(6) 1_455 ?
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.97(3)
2 0.03(3)
